thermal expansion of beryllium and aluminum-beryllium alloys · pdf file 2012. 11....
Click here to load reader
Post on 28-Feb-2021
Embed Size (px)
THERMAL EXPANSION OF BERYLLIUM AND ALUMINUM- BERYLLIUM ALLOYS
By Peter Hidnert and W. T. Sweeney
The investigation described in this paper was undertaken because no data on the thermal expansion of beryUium or any of its alloys were available. The paper gives results on the linear thermal expansion of beryllium (98.9 per cent)
and five aluminum-beryllium alloys containing various percentages of beryllium (4 to 33 per cent). Expansion determinations were made over various tem- perature ranges, between —120 and +700° C. on a sample of beryllium, and between room temperature and 500° C. on the aluminum-beryllium alloys. The expansion curves of beryllium and aluminum-beryllium alloys are shown and discussed.
The average coefficient of expansion of beryllium is 12.3X10"^ per degree centigrade between 20 and 100° C. Beryllium expands considerably less than the other elements of subgroup IIB (magnesium, zinc, cadmium, and mercury). The coefficients of expansion of the aluminum-beryllium alloys decrease with
increase in the beryllium content. On a second heating the coefficients are generally larger than the corresponding values obtained in the first heating.
The relations between the coefficients of expansion and the chemical composition were compared with the equilibrium diagram obtained by Oesterheld, and were found to be in agreement with the theory.
Figure 10 shows a comparison of the expansion curves of beryllium (98.9 per
cent) and the aluminum-beryllium alloys between room temperature and 500° C. The table in the summary gives a resume of average coefficients of expansion derived from the data on all samples for various temperature ranges between 20 and 500° C.
I. Introduction 533
II. Materials investigated 534 III. Apparatus 536 IV. Results 536
1. BeryUium (98.9 per cent) 536 2. Aluminum-beryllium alloys 538
V. Summary 543
In view of the fact that there was no available information on the thermal expansion of berylhum or any of its alloys, an investigation was recently undertaken to supply data ^ on this metal and some of its alloys.
1 Some preliminary data on beryllium were presented by the authors to the American Physical Society on Feb. 26, 1927 (Phys. Rev., 29, p. 616; 1927).
534 Scientific Papers of the Bureau oj Standards [ voi. a
This paper gives the results of the investigation on the linear
thermal expansion of beryllium and five aluminum-beryllium alloys containing various percentages of beryllium (between 4 and 33 per cent). Expansion determinations were made over various tempera- ture ranges between —120 and +700° C. on a sample of beryllium and between room temperature and 500° C. on the aluminum- beryllium alloys. Five tests were made on the specimen of beryllium and two tests on each of the aluminum-beryllium alloys. The authors wish to express their appreciation for the cooperation
b}^ the BerylHum Corporation of America, Cleveland, Ohio. This company furnished the samples of beryllium and aluminum-beryllium alloys, and information about the preparation. Acknowledgment is due to H. W. Bearce, W. Souder, and H. W. Gillett, Bureau of Standards, for valuable suggestions.
II. MATERIALS INVESTIGATED
One sample of cast beryllium and five samples of cast aluminum- beryllium alloys (4 to 33 per cent beryllium) were investigated.
Each sample was approximately 300 mm in length and 10 mm in diameter.
The following information relating to the casting of beryllium was furnished by the manufacturer:
In melting and casting beryllium our practice has been first to prepare a flux composed of about 10 per cent barium fluoride and 90 per cent barium chloride. This flux after fusion and cooling is ground to a fine powder. The buttons of massive beryllium are placed in a graphite crucible and a small amount of this powdered flux sprinkled on the surface. The crucible ia then covered with just the ordinary graphite cover and heated to about 1,350 or 1,400° C. in a gas furnace. About 5 or 10 minutes before pouring it is advisable to remove the cover and rotate the crucible in order to bring all the particles of metal together in one fluid mass. It is then superheated for about 10 minutes longer and rapidly cast. We might add that in the melting of small amounts, such as 10 to 25 g, some losses are sustained, but in handling larger amounts we have been able to get practically 100 per cent recovery in this manner.
The Beryllium Corporation of America states that virgin alumi- num and beryllium containing about 99 per cent beryllium were used in the preparation of the aluminum-beryllium alloys. Iron was the chief impurity in beryllium. The cast alloys were prepared by heat- ing the two metals (aluminum and beryllium) to about 1,100 to 1,200° C. with a small amount of the fluoride-chloride flux mentioned in the preceding paragraph.
For information about other methods of preparing beryllium and its alloys the reader should refer to recent papers ^ on this subject.
» Hopkins and Meyer, The electrolytic production of beryllium, Trans. Am._ Electrochem. Soc, 45, p. 475; 1924. Engle and Hopkins, The metallurgy and alloys of berj-ilium, Trans. Am. Electrochem. Soc, 45, p. 483; 1924. Vivian, Beryllium, Trans. Faraday Soc, 2% p. 211; 1926.
Sweeneyj Beryllium and Aluminum-Beryllium Alloys 535
Table 1 gives the chemical composition and the densities of the
samples investigated. In the alloys the iron impurity increases
regularly with the beryllium content.
Chemical composition and densities of beryllium and aluminum- beryllium alloys 1
Chemical analyses 2 Density 3
Sample Alumi- num
Silicon Copper Iron Manga- nese
in g/cm 3 at20°C.
1223 < Beryllium' Per cent
66.3 71.9 81.0 89.7 95.7
Per cent 98.9 32.7 27.5 18.6 10.1 4.2
Per cent 0.18 .11 .10 .12 .12 .10
Per cent 0.06 .09 .08 .11 .09 .10
Per cent 0.90 .84 .58 .36 .19 .12
Per cent 0.20 .06 .05 .05 .01 .01
1224... 1226.. - 1226
Aluminum-beryllium alloy do do
? 2. 225 8 2. 202 2.242
do... - . do
1 The chemical analyses and the densities were determined after the expansion measurements were made on the samples.
* Determined by J. A. Scherrer, of this bureau. Magnesium, calcium, lead, zinc, nickel, and selenium were not detected.
3 Determined by Miss E. E. Hill, of the volumetric section of this bureau. * Dr. W. F. Meggers, of this bureau, made a spectrochemical analysis of this sample by means of its
spark spectrum. The following additional impurities were found: Chromium, selenium, aluminum, mag- nesium, calcium, silver (trace), and bismuth (doubtful).
« The electrical resistivity of this rod of beryllium was determined under the direction of Dr. F. Wenner, of this bureau, and found to be 10.2 microhm-cm at 21.5° C. Assuming the resistivity temperature coefficient to be 0.004 per degree centigrade, the resistivity at 20° C. is 10.1 microhm-cm. The value given is probably not in error by as much as 6 per cent,
6 Not detected. ^ On a second determination the density was found to be 2.224 g/cm^ at 29° C. 8 After this density determination the sample was cut into two pieces and additional density determina-
tions were made. The density of these pieces was found to be 2.205 and 2.196 g/cm^ at 25° C.
Since there are but few data available on the mechanical prop- erties ^ of beryllium and beryllium-aluminum alloys, an attempt
was made ^ to determine the tensile properties and hardness of the specimens after the expansion data had been obtained. However, due to the presence of blowholes and inclusions, satisfactory tensile data were not obtained.
It is of interest to note that all the alloys machined readily, although the length of chip decreased rapidly with increasing beryllium content.
Kerosene was very beneficial in obtaining a good finish. The beryllium sample could not be machined but was readily ground. The results of the hardness tests are given in Table 2. The
hardness was not very uniform. Each value given is the average of four determinations.
Hardness of beryllium and alumium-beryllium alloys
. Material Beryl- lium
Sample (Baby) Brinell °
Rock- well 6
1223 Beryllixma Per cent
98.9 32.7 27.6 18.6 10.1 4.2
153 48 37 28 32 34
113 1224 Aluminum-beryllium alloy 76 1225.. do 63 1226 do 42 1227... do 37 1228 do 36
o 6.4 kg load on 1.6 mm ball (equivalent to 250 kg load on 10mm ball)
*> A one-eighth Inch ball, 60 kg load. These Rockwell hardness numbers are arbitrary and show only relative hardness.
8 Kroll, Metall. u. Erz, 33, p. 616; 192G; or The Metal Industry, London, 30, p. 645; 1927. * Under the direction of J. R. Freeman, jr., of the metallurgical division of this bureau.
536 Scientific Papers of the Bureau of Standards [ voi. 22
Micrographs ^ showing the structure of the materials investigated
are given in Figure 1. No unusual features were noted in the micro- structure. A number of cavities were observed in all of the speci- mens.
Figure 1 of Bureau of Standards Scientific Paper No. 524 (vol. 21, p. 1; 1926) shows part of the apparatus used in this investigation.